Abstract
We show that certain threedimensional (3D) superlattice nanostructure based on Bi_{2}Te_{3} topological insulator thin films has better thermoelectric performance than twodimensional (2D) thin films. The 3D superlattice shows a predicted peak value of ZT of approximately 6 for gapped surface states at room temperature and retains a high figure of merit ZT of approximately 2.5 for gapless surface states. In contrast, 2D thin films with gapless surface states show no advantage over bulk Bi_{2}Te_{3}. The enhancement of the thermoelectric performance originates from a combination of the reduction of lattice thermal conductivity by phononinterface scattering, the high mobility of the topologically protected surface states, the enhancement of Seebeck coefficient, and the reduction of electron thermal conductivity by energy filtering. Our study shows that the nanostructure design of topological insulators provides a possible new way of ZT enhancement.
Background
The search of good thermoelectrics with high figure of merit [1,2]
is usually baffled by the competition of the Seebeck coefficient S, the electrical conductivity σ, the electron thermal conductivity κ_{e} and the lattice thermal conductivity κ_{l}. Recent discoveries that some of the best thermoelectric materials such as Bi_{2}Te_{3}[1] are also strong 3D topological insulators [35], and experimental studies of the mechanical exfoliation and growth of quintuple layers (QL, 1 QL ≈ 0.748 nm) of Bi_{2}Te_{3}[6,7] attract much interest [811] in the thermoelectric properties of thin films of Bi_{2}Te_{3} with one or a few QL.
High ZT values of Bi_{2}Te_{3} thin films depend crucially on the opening of a subgap at the surface, which disappears quickly with the increasing of the film thickness, as suggested both theoretically [1214] and experimentally [15,16]. Relatively accurate density functional theory calculations [16,17] show that the (indirect) surface gap of Bi_{2}Te_{3} vanishes as soon as the thickness of the thin film increases to 3QL. Despite the high mobility [18] of the surface electrons, the gapless surface states would lead to poor thermoelectric performance due to low Seebeck coefficient and high electron thermal conductivity. However, by creating suitable nanostructures, extra energydependent electron scattering mechanisms can be introduced, which could increase the Seebeck coefficient [19,20] and reduce the electron thermal conductivity. The consideration of nanostructures of thin films is also motivated by the fact that a single layer of thin film is not of much practical use for thermoelectric applications, and stacks of thin films have much lower lattice thermal conductivity compared with the bulk [21].
In this paper, we propose a 3D superlattice nanostructure based on thin films of Bi_{2}Te_{3} topological insulator, with one thin film (thickness a) and one stripeshaped layer (thickness c along the z direction and width b along the x direction) stacked alternatively; the spacing between two nearby stripes is d, as shown in Figure 1. The system is considered to be infinite along the y direction and periodic in the x and z directions. We are interested in thermoelectric transport along the x direction. Along the transport direction, the surface carriers will encounter potential barriers/wells if the surface gap is different from the bulk gap. We will give a comparison study of the thermoelectric properties of 2D thin films and the 3D superlattice and show that the latter has higher ZT values due to the enhanced Seebeck coefficient and reduced electron thermal conductivity through energy filtering as well as the reduced lattice thermal conductivity by interface phonon scattering. More importantly, the 3D superlattice shows high ZT values even when the surface states are gapless, in which case 2D thin films have low ZT values.
Figure 1. A sketch of the physical system to be studied. The system can be regarded as a 3D superlattice with one thin film (thickness a) and one stripeshaped layer (thickness c along the z direction and width b along the x direction) stacked alternatively; the spacing between two adjacent stripes is d. The transport direction is along the x axis.
The 3D superlattice structure proposed here can be regarded as bulk Bi_{2}Te_{3} which is nanoporous and resembles nanoporous Si [22] and nanoporous Ge [23], both of which show significant enhancement of the figure of merit due to orders of magnitude reduction in the lattice thermal conductivity. The difference is that the electronic transports for nanoporous Bi_{2}Te_{3} and Si/Ge are dominated by surface and bulk carriers, respectively.
Methods
We first consider the lattice thermal conductivity which depends on the geometric parameters and can be estimated using the modified effective medium approximation [24] which treats the system as a nanocomposite. In our case, we can perceive the system as a nanocomposite with vacuum (hole) included in the bulk phase. Taking the thermal conductivity of the holes to be zero, we can express the effective lattice thermal conductivity of the 3D superlattice along the x direction as
where K_{b} and Λ_{b} are lattice thermal conductivity and phonon mean free path (MFP) for the bulk phase,
respectively;
A comparison with nanoporous Si [22] and Ge [23] is helpful. While the values of lattice thermal conductivities for bulk Bi_{2}Te_{3}, Ge and Si range from a few watts per meter Kelvin to several hundred watts per meter Kelvin, the values for the corresponding nanoporous materials are all reduced to below 1 W/(m K). This fact is another indication of the dominance of phononinterface scattering over the phononphonon scattering.
We then consider electron transport coefficients. Since the system is considered to be infinite, the electronic transport is diffusive and Boltzmann's formalism applies. By solving the Boltzmann transport equations with the relaxation time approximation, one can express the thermoelectric transport coefficients as [28]
where e is the magnitude of the elementary charge, T is the absolute temperature, μ is the chemical potential, and the integrals (f is the FermiDirac distribution)
are functionals of the transport distribution function (TDF) [29,30]
which are determined by the electronic structure and the electron scattering mechanisms of the material. For simple band structure, the TDF is a product of density of states g(E), velocity square along the transport direction v_{x}(E)^{2}, and electron relaxation time τ(E):
The electronic structures of thin films of topological insulator differ significantly from that of the bulk. First, as the thickness of the film is reduced to one or a few QL, the spinpolarized surface states at one surface will mix up with the components of the opposite spin from the other surface and lead to a hybridization gap at the Dirac point to avoid the crossing of bands with the same quantum number [1217]. Second, at this thickness, the layers underneath the film surface should be treated as quantum well, which is indicated by experimental observations [15]. In this paper, we adopt a simple parameterization [8] of the dispersion relation of the surface states
where ‘±’denotes the conduction (valance) band, V_{D} of approximately 4 × 10^{5} m/s [4,18] is the Dirac velocity, and 2 ∆_{f} is the surface gap. The zero of energy is chosen to be at the center of the surface gap. This simple dispersion relation is derived from symmetry arguments [8] and exhibits the essentials of thermoelectric properties of the surface states. From the above dispersion relation, we can express the velocity square along the transport direction and the effective 3D density of states for a thin film with thickness a as
For the 3D superlattice structure, the square of velocity along the transport direction takes the same form as in Equation 10, and the effective 3D density of states is that of Equation 11 as scaled by a/(a + c). Since the quantum well states lie much above, we can safely disregard them and consider the surface states only. We also only consider the conduction band with E > 0.
To compute the electronic transport coefficients, we should also find an estimation of the electron relaxation time. Experimental studies [18] show that the surface electron mobility μ_{s} of Bi_{2}Te_{3} approaches 10^{4} cm^{2} V^{−1} s^{−1}, about an order of magnitude higher than the bulk value. We use this experimental value of mobility to calculate the intrinsic surface electron relaxation time τ_{s}. For the superlattice, the surface carriers also encounter potential barriers/wells whenever they reach the boundaries of the surfaces (located at the crossing lines between the thin films and the strips) and suffer from additional scattering. The strips are modeled by rectangular potential barriers/wells with height V_{i} = Δ_{b} − Δ_{f} and width b and average distance L = b + d. Let the transmission probability for the charge carriers with energy E through a single strip be P(E). The path length after passing through the nth strip and scattering by the (n + 1)th one is nLP(E)^{n}(1 − P(E)). The mean free path is the sum of all of the possible path lengths [31], ∑ _{n = 1}^{∞}nLP(E)^{n}(1 − P(E)) = LP(E)/(1 − P(E)). The corresponding additional relaxation time τa is the mean free path divided by the velocity,
The transmission probability P(E) is determined by the interface potential barrier/well according to the following standard quantum mechanical calculations:
The total surface electron relaxation time τ for the superlattice is given by
This method of calculating the total electron relaxation time has been recently applied to the study of thermoelectric properties of nanocomposites [32,33]. We assume 2Δ_{b} = 0.15 eV for bulk Bi_{2}Te_{3} according to the experimental value [34]. The surface gap is chosen to be 2Δ_{f} = 0.3, 0.06, and 0 eV for thin films with thickness 1QL, 2QL, and 3QL, respectively, as suggested by firstprinciple calculations [17]. The effective mass m^{*} entering Equation 13 stands for that of bulk Bi_{2}Te_{3}, which has a highly anisotropic effective mass tensor, with the inplane components 0.021 m_{0} and 0.081 m_{0} and the outofplane component 0.32 m_{0} (m_{0} is the mass of a free electron) [35]. For simplicity, we take m^{*} to be 0.1 m_{0} in our calculations. The exact value of m^{*} is not very crucial for our discussions, since it only affects the optimal value of b.
Results and discussion
Figure 3 shows the calculated ZT values for 2D thin films and the 3D superlattice with varying geometric parameters. Both of the standalone thin film with thickness of 1 QL and the 3D superlattice with a = 1QL exhibit high figure of merit ZT of 5 to 6 at room temperature with appropriate doping level. For thicker films, the surface gap becomes smaller and yields lower ZT values. However, the 3D superlattice is much more robust against the disappearance of surface gap and still shows peak value of ZT of approximately 2.5 (Figure 3f) for gapless states. In contrast, a gapless thin film with a thickness of 3QL demonstrates no better performance than the bulk material (Figure 3e).
Figure 3. Figure of merit. ZT values as functions of temperature and chemical potential for Bi_{2}Te_{3} 2D thin films with thickness 1QL (a), 2QL (c), and 3QL (e); and the 3D superlattice with a = 1QL (b), 2QL (d) and 3QL (f). For the a = 1QL case, c = 1QL, b and d = 10 nm; for the a = 2QL case, c = 2QL, b = 7.5 nm and d = 10 nm; for the a = 3QL case, c = 3QL, b = 7.5 nm and d = 10 nm. The zero of energy is chosen to be at the center of the surface gap.
ZT values depend on the geometric parameters a, b, c and d since both the lattice thermal conductivity and the electronic transport coefficients depend on these parameters. The dependence of ZT on the geometric parameters for a = 3QL case is shown in Figure 4. While ZT has a weak dependence on d, it depends strongly on b since this parameter largely affects the transmission probability P(E) and hence the electron relaxation time. Only an appropriate b gives the desired energy filtering effect. The weak dependence of ZT on d results from the fact that the phonon collision probability 1/Λ_{c} and the hole volume fraction ϕ have opposite dependences on d and the fact that the total electron relaxation time is not strongly dependent on d. The optimized value of c results from the optimization of the B factor [36] which represents the relative transport strength of electrons over phonons. A large value of c gives a lower lattice thermal conductivity and a lower effective 3D density of states, and only an appropriate value of c gives an optimized B factor. We should note that our model is only valid for appropriate ranges of these geometric parameters. For example, our model cannot be extrapolated to the c = 0 case, since in this limiting case, our model treats the system as parallel thin films with vanishing separation rather than the bulk material. The conclusion of this parametric study leads to the following recommendations for the relevant parameters: c takes the same value of a, b takes the value of 5–10 nm, and d takes the value of 10–20 nm.
Figure 4. Optimized geometric parameters. Optimization of the geometric parameters b, c, and d for the 3D superlattice with a = 3QL at T = 250 K and μ = 60 meV. The geometric parameter dependence of ZT values for 3D superlattice with a = 2QL and 1QL has similar trends as given here for the case of a = 3QL.
To understand why 3D superlattice outperforms 2D thin films, we plot in Figure 5 the individual thermoelectric transport coefficients as functions of chemical potential
at T = 250 K for the case of a = 3QL, where the difference of the ZT values is most significant. As expected, the electrical conductivity of the superlattice
is heavily reduced (Figure 5a) due to the additional scattering by the potential barriers/wells. The additional
scattering reduces the effective mobility of charge carriers and decreases the electrical
conductivity. This reduction of electrical conductivity is not desirable for obtaining
high figure of merit. However, this additional scattering also has two beneficial
effects on thermoelectric transport, which result in an increase of the Seebeck coefficient
and a decrease of the electronic thermal conductivity. Firstly, the additional relaxation
time is strongly energy dependent in such a way that charger carriers with energies
lower than a certain value are largely scattered back and those with energies higher
than a certain value mostly transport through. With an appropriate choice of the barrier/well
width b and the chemical potential, one can effectively filter out the charge carriers with
energies lower than the chemical potential. Since charger carriers with energies above
and below the chemical potential contribute oppositely to the Seebeck coefficient
(Equation 4), this energyfiltering mechanism can significantly enhance the Seebeck
coefficient (Figure 5b). Whether the power factor is increased or decreased due to this energy filtering
effect depends on the choices of relevant parameters. In the present case, the power
factor is decreased (Figure 5c). From Figure 3e,f, we can infer the optimal chemical potential as about 65 meV. At this value of chemical
potential, the power factor for the 2D thin film is about twice as large as that for
the 3D superlattice. Then, why does the figure of merit for superlattice reach a value
of about 2.5, while that for the thin film only takes a value of about 0.6? This is
mainly resulted from the significant reduction of the electronic thermal conductivity
for the superlattice compared with the thin film. As can be seen from Figure 5d, the electronic thermal conductivities for the thin film and the superlattice are
about 13 and 1 W/(m K) respectively. Combined with the reduction of the lattice thermal
conductivity, the total thermal conductivity for the superlattice is about 1/8 of
that for the thin film. A combination of all these effects results in a fourfold
enhancement of the ZT for the superlattice compared with the thin film. The significant reduction of the
electronic thermal conductivity also results from the energy filtering mechanism.
With the filtering of the lowenergy charger carriers, the energy distribution of
transport distribution function [29,30] becomes more concentrated, resulting in a violation of the WiedemannFranz law [28] which states that the electronic thermal conductivity is proportional to the electrical
conductivity, κ_{e} = L_{0}σT, with the Lorentz number
Figure 5. Thermoelectric transport coefficients. Thermoelectric transport coefficients as functions of chemical potential at T = 250 K for the 2D thin film with thickness 3QL and the 3D superlattice with a = 3QL, b =7.5 nm, and c = 3QL, d = 10 nm.
To get an intuition of the necessity of violating the WiedemannFranz law for superior thermoelectric performance, suppose that the lattice thermal conductivity is reduced to zero, and the Seebeck coefficient is 200 μVK^{−1}, then if the WiedemannFranz law were strictly valid, we would have achieved a relatively low figure of merit ZT = S^{2}/L_{0} ≈ 1.6 regardless how large the electrical conductivity would be. Thus, as we approach the lower limit of lattice thermal conductivity, it is imperative to find a way to change the shape of the transport distribution function [29,30] either by altering the electronic structures [38] or by introducing energydependent electron scattering mechanisms.
Finally, we add some view points on the approach that we used in this work. For the study of thermoelectric transport of a nanostructured material, there are two complementary ways of viewing the system. One is to take the system as a whole, in which case the nanostructures do alter the electronic structure of the system, but it is difficult to calculate the band structure of such large system directly by first principles method due to large number of atoms presented in nanostructures. Another way is to view the system as some bulk material with nanostructures that do not affect the electronic structure of the bulk material significantly, but introduce some extra scatterings for the charge carriers. We have chosen the second approach in our study. This approach has been widely used in the community of thermoelectrics. For example, in the study of nanocomposites with grain boundaries [32,33], one usually assumes that the electronic structure inside the grain boundary is the same as that of the corresponding bulk material. The grain boundary does not affect significantly the energyband structure and only serves as a scattering interface. The only difference between our model and the nanocomposite models [32,33] is that our bulk material is quasitwodimensional instead of threedimensional, and the grain boundaries are replaced by the strips in our proposed structure. So long as the average distance between the strips is large compared with the size of the strips (which is the case for the optimized structures), this view point is valid and there is no significant deficiency in our model.
Conclusions
In summary, we demonstrated that certain nanostructures of topological insulators have the potential of overcoming the obstacle of competition of the individual thermoelectric transport coefficients to achieve high thermoelectric figure of merit. High electron mobility of the topologically protected surface states together with the holy structure of the 3D superlattice ensures a large B factor [36], and the energy filtering effect introduced by the inhomogeneous superlattice structure promotes the Seebeck coefficient and the ratio of electrical conductivity to the electron thermal conductivity. The optimal temperature of performance for the 3D superlattice with optimized geometric parameters is around or below room temperature, making it very appealing for thermoelectric power generation and refrigeration applications around and below room temperature, respectively. In addition, a similar structure has appeared in a thin film transistor array, with an insulating substrate and a stripeshaped semiconductor layer for a plurality of transistors [39], which demonstrates the experimental feasibility of our proposed 3D superlattice structure. The detailed information of geometric and electronic properties of the fabricated superlattice can be characterized by integrated electron scattering and Xray scattering techniques [40,41].
Competing interests
The authors declare that they have no competing interests.
Authors' contributions
ZF carried out the main part of the calculations and drafted the manuscript. JZ carried out part of the calculations. HQW participated in the organization of the project and discussions of the results and revised the manuscript. JCZ organized the project, analyzed the results and revised the manuscript. All authors read and approved the final manuscript.
Acknowledgements
This work is supported by the Minjiang Scholar Distinguished Professorship Program through Xiamen University of China, Specialized Research Fund for the Doctoral Program of Higher Education (grant numbers 20090121120028 and 20100121120026), Program for New Century Excellent Talents in University (NCET) (grant number NCET090680) and the National Science Foundation of China (grant number U1232110).
References

Goldsmid HJ: Thermoelectric Refrigeration. New York: Plenum; 1964.

Zheng JC: Recent advances on thermoelectric materials.
Front Phys China 2008, 3:269279. Publisher Full Text

Zhang H, Liu C, Qi X, Dai X, Fang Z, Zhang S: Topological insulators in Bi2Se3, Bi2Te3and Sb2Te3with a single Dirac cone on the surface.
Nature Phys 2009, 5:438442. Publisher Full Text

Chen Y, Analytis J, Chu J, Liu Z, Mo S, Qi X, Zhang H, Lu D, Dai X, Fang Z, Zhang S, Fisher I, Hussain Z, Shen Z: Experimental realization of a threedimensional topological insulator, Bi2Te3.
Science 2009, 325:178181. PubMed Abstract  Publisher Full Text

Hsieh D, Xia Y, Qian D, Wray L, Dil JH, Meier F, Osterwalder J, Patthey L, Checkelsky JG, Ong NP, Fedorov AV, Lin H, Bansil A, Grauer D, Hor YS, Cava RJ, Hasan MZ: A tunable topological insulator in the spin helical Dirac transport regime.
Nature 2009, 460:11011105. PubMed Abstract  Publisher Full Text

Teweldebrhan D, Goyal V, Balandin AA: Exfoliation and characterization of bismuth telluride atomic quintuples and quasitwodimensional crystals.
Nano Lett 2010, 10:12091218. PubMed Abstract  Publisher Full Text

Teweldebrhan D, Goyal V, Rahman M, Balandin AA: Atomicallythin crystalline films and ribbons of bismuth telluride.
Appl Phys Lett 2010, 96:053107. Publisher Full Text

Ghaemi P, Mong RSK, Moore JE: Inplane transport and enhanced thermoelectric performance in thin films of the topological insulators Bi2Te3and Bi2Se3.
Phys Rev Lett 2010, 105:166603. PubMed Abstract  Publisher Full Text

Qiu Q, Ruan X: Thermal conductivity prediction and analysis of fewquintuple Bi2Te3thin films: a molecular dynamics study.
Appl Phys Lett 2010, 97:183107. Publisher Full Text

Zahid F, Lake R: Thermoelectric properties of Bi2Te3atomic quintuple thin films.
Appl Phys Lett 2010, 97:212102. Publisher Full Text

Tretiakov QA, Abanov A, Sinova J: Holey topological thermoelectrics.
Appl Phys Lett 2011, 99:113110. Publisher Full Text

Linder J, Yokoyama T, Sudb A: Anomalous finite size effects on surface states in the topological insulator Bi2Se3.

Liu C, Zhang H, Yan B, Qi X, Frauenheim T, Dai X, Fang Z, Zhang S: Oscillatory crossover from twodimensional to threedimensional topological insulators.

Lu H, Shan W, Yao W, Niu Q, Shen S: Massive Dirac fermions and spin physics in an ultrathin film of topological insulator.

Zhang Y, He K, Chang C, Song C, Wang L, Chen X, Jia J, Fang Z, Dai X, Shan W, Shen S, Niu Q, Qi X, Zhang S, Ma X, Xue Q: Crossover of the threedimensional topological insulator Bi2Se3to the twodimensional limit.
Nat Phys 2010, 6:584588. Publisher Full Text

Li Y, Wang G, Zhu X, Liu M, Ye C, Chen X, Wang Y, He K, Wang L, Ma X, Zhang H, Dai X, Fang Z, Xie X, Liu Y, Qi X, Jia J, Zhang S, Xue Q: Intrinsic topological insulator Bi2Te3thin films on Si and their thickness limit.
Adv Mater 2010, 22:40024007. PubMed Abstract  Publisher Full Text

Park K, Heremans JJ, Scarola VW, Minic D: Robustness of topologically protected surface states in layering of Bi2Te3thin films.
Phys Rev Lett 2010, 105:186801. PubMed Abstract  Publisher Full Text

Qu D, Hor YS, Xiong J, Cava RJ, Ong NP: Quantum oscillations and Hall anomaly of surface states in the topological insulator Bi2Te3.
Science 2010, 329:821824. PubMed Abstract  Publisher Full Text

Vashaee D, Shakouri A: Improved thermoelectric power factor in metalbased superlattices.
Phys Rev Lett 2004, 92:106103. PubMed Abstract  Publisher Full Text

Zeng G, Zide JMO, Kim W, Bowers JE, Gossard AC, Bian Z, Zhang Y, Shakouri A, Singer SL, Majumdar A: Crossplane Seebeck coefficient of ErAs:InGaAs/InGaAlAs superlattices.
J Appl Phys 2007, 101:034502. Publisher Full Text

Goyal V, Teweldebrhan D, Balandin AA: Mechanicallyexfoliated stacks of thin films of Bi2Te3topological insulators with enhanced thermoelectric performance.
Appl Phys Lett 2010, 97:133117. Publisher Full Text

Lee JH, Galli GA, Giulia A, Grossman JC: Nanoporous Si as an efficient thermoelectric material.
Nano Lett 2008, 8:37503754. PubMed Abstract  Publisher Full Text

Lee JH, Grossman JC: Thermoelectric properties of nanoporous Ge.
Appl Phys Lett 2009, 95:013106. Publisher Full Text

Minnich A, Chen G: Modified effective medium formulation for the thermal conductivity of nanocomposites.
Appl Phys Lett 2007, 91:073105. Publisher Full Text

Jeong C, Datta S, Lundstrom M: Full dispersion versus Debye model evaluation of lattice thermal conductivity with a Landauer approach.
J Appl Phys 2011, 109:073718. Publisher Full Text

Kaibe H, Tanaka H, Sakata M, Nishida I: Anisotropic galvanomagnetic and thermoelectric properties of ntype Bi2Te3single crystal with the composition of a useful thermoelectric cooling material.
J Phys Chem Solids 1989, 50:945950. Publisher Full Text

Tedenac JC, Corso SD, Haidoux A: Growth of bismuth telluride thin films by hot wall epitaxy, thermoelectric properties. In Symposium on Thermoelectric Materials 1998–the Next Generation Materials for SmallScale Refrigeration and Power Generation Applications: November 30December 3 1998; Boston. 93rd edition. Boston: Materials Research Society; 1998.

Ashcroft NW, Mermin ND: Solid State Physics. Orlando, Florida: Saunders College Publishing; 1976.

Mahan GD, Sofo JO: The best thermoelectric.
Proc Natl Acad Sci USA 1996, 93:74367439. PubMed Abstract  Publisher Full Text  PubMed Central Full Text

Fan Z, Wang HQ, Zheng JC: Searching for the best thermoelectrics through the optimization of transport distribution function.
J Appl Phys 2011, 109:073713. Publisher Full Text

Atakulov SBA, Shamsiddnov AN: The problem of transport phenomena in polycrystalline semiconductor thin films with potential barriers in the case where the carriers gas degenerated.
Solid State Commun 1985, 56:215219. Publisher Full Text

Popescu A, Woods LM, Martin J, Nolas GS: Model of transport properties of thermoelectric nanocomposite materials.

Zhou J, Li X, Chen G, Yang R: Semiclassical model for thermoelectric transport in nanocomposites.

Thomas GA, Rapkine DH, Dover RBV, Mattheis LF, Surden WA, Schneemaper LF, Waszczak JV: Large electronicdensity increase on cooling a layered metal: Doped Bi2Te3.
Phys Rev B 1992, 46:15531556. Publisher Full Text

Landolt HH, Bornstein R: Numerical Data and Functional Relationships in Science and Technology, New Series. Vol. 17f edition. Berlin: SpringerVerlag; 1983:272278.

Hicks LD, Dresselhaus MS: Effect of quantumwell structures on the thermoelectric figure of merit.
Phys Rev B 1993, 47:1272712731. Publisher Full Text

Humphrey TE, Linke H: Reversible thermoelectric nanomaterials.
Phys Rev Lett 2005, 94:096601. PubMed Abstract  Publisher Full Text

Heremans JP, Jovovic V, Toberer ES, Saramat A, Kurosaki K, Charoenphakdee A, Yamanaka S, Snyder GJ: Enhancement of thermoelectric efficiency in PbTe by distortion of the electronic density of states.
Science 2008, 321:554557. PubMed Abstract  Publisher Full Text

Matsubara R, Ishizaki M: Thin film transistor array, method for manufacturing the same, and active matrix type display using the same.
2008.
US patent No. 0197348 A1.8 Feb 2008

Zheng JC, Wu L, Zhu Y: Aspherical electron scattering factors and their parameterizations for elements from H to Xe.
J Appl Cryst 2009, 42:10431053. Publisher Full Text

Zheng JC, Frenkel AI, Wu L, Hanson J, Ku W, Bozin ES, Billinge SJL, Zhu Y: Nanoscale disorder and local electronic properties of CaCu3Ti4O12: an integrated study of electron and xray diffraction, xray absorption fine structure and first principles calculations.